Finite Element Analysis of Delamination in Woven Composites under QuasiStatic Indentation


 Chloe York
 1 years ago
 Views:
Transcription
1 Copyright 2013 Tech Science Press CMC, vol.35, no.1, pp.6785, 2013 Finite Element Analysis of Delamination in Woven Composites under QuasiStatic Indentation M. C. Song 1, B.V. Sankar 1, G. Subhash 1, C. F. Yen 2 Abstract: Delamination initiation and propagation in plain woven laminates and 3D orthogonal woven composites during short beam shear (SBS) test were analyzed using finite element (FE) analyses. Two kinds of 3D woven composites, containing single zyarns and double zyarns, were considered. The FE models were guided by experimental observations from SBS tests for the same material systems. A series of mechanisms including creation and evolution of matrix cracks and delaminations were modeled discretely. The forcedisplacement curves obtained from the FE simulations were compared with those from experiments. Further parametric studies were conducted to investigate the effects of zyarns and interlaminar fracture toughness on delamination in woven composites. The results from the FE simulations revealed that zyarns in 3D woven composites can play a major role in impeding propagation of interlaminar cracks. On the other hand 2D plain woven laminates without any zreinforcement demonstrated higher interlaminar fracture toughness due to undulation in yarns. 3D woven composites with double yarns showed better damage tolerance than single yarn 3D woven composites and their behavior was very similar to composite laminates with high interlaminar fracture toughness. Keywords: 3D woven composites, plain woven laminate, FEM cohesive element, delamination 1 Introduction Prediction of damage and failure in laminated composite materials is one of the significant considerations in the design and operation of composite structures in various applications such as aerospace structures and military equipment. Among the various damage modes delamination is the most serious one as it leads to severe stiffness loss of the structures. Various methods for arresting crack growth 1 University of Florida, Gainesville, FL, USA. 2 US Army Research Laboratory, Aberdeen Proving Ground, MD, USA.
2 68 Copyright 2013 Tech Science Press CMC, vol.35, no.1, pp.6785, 2013 due to delamination have been suggested, e.g. [Sankar and Sharma (1997); Jain and Mai (1998); Chen, Sankar and Ifju (2002); Cartie (2000)]. One of those is to embed trans laminar reinforcements (TLRs) into the composite. Among several manufacturing processes used to include TLRs, 3D weaving process has substantial advantage over stitching or zpinning in that the traditional weaving machines can be readily utilized. Numerous experimental [Sankar and Sharma (1997); Jain and Mai (1998); Chen, Sankar and Ifju (2002); Cartie (2000)], numerical[cartie (2000); Dantuluri, Maiti, Geubelle, Patel and Kilic (2007); Grassi and Zhang (2003); Ratcliffe and Kruger (2006); Sankar and Hu(1991)] and analytical studies [Sankar and Dharmapuri (1998); Sridhar, Massabo, Cox and Beyerlein (2002); Ratcliffe and O Brien (2004); Robinson and Das (2004); Mabson and Deobald (2000); Byrd and Birman (2005); Song, Sankar, Subhash and Yen (2012); Sankar and Zhu (2000)] have been conducted to determine the effect of TLRs on delamination of composites. Walter et al. [Walter, Subhash, Sankar and Yen (2010)] has tested different types of woven composites using short beam shear (SBS) test, and reported that the amount and type of zyarns can influence the damage characteristics of composites. Our goal in the present study is to evaluate the effect of zyarn, on suppressing the delamination propagation and thus enhancing the damage tolerance of composites using finite element (FE) simulations. Resistance against crack development can be quantified by apparent fracture toughness expressed in terms of inherent interlaminar fracture toughness and the additional energy required due to bridging effect [Walter, et al., (2010)]. The influences of both these terms on delamination were analyzed using finite element method (FEM). We selected three different types of specimens; single and double yarn 3D woven composites, denoted as SY3W and DY3W, respectively, and 2D plain woven laminated composite (2DPL) for this study. The effects of zyarn and inherent interlaminar fracture toughness on damage tolerance were investigated by comparing the loaddeflection behavior SY3W and the DY3W to the 2DPL specimen and varying inherent interlaminar fracture toughness of the 2DPL in a parametric study. It is well known that matrix cracks precede delamination when a laminated composite beam/plate is subjected to a quasistatic indentation or an impact load [Sankar and Sun (1986)]. Walter et al. [Walter, Subhash, Sankar and Yen (2010)] performed short beam shear tests on 3D woven glass/epoxy composites to understand the damage initiation and propagation mechanisms under impact loads. The experiments showed that matrix cracks initiated in resin pockets between the zyarns and also in the weft yarns parallel to the yaxis (see Fig. 1). Optical micrographs also showed short delaminations and crushing failure beneath the indenter. However, these failures were highly localized beneath the indenter. On the other hand, the delaminations emanating from matrix cracks significantly changed the global
3 Finite Element Analysis of Delamination 69 response of the specimens by reducing their stiffness significantly. In fact the interaction of matrix cracks and delaminations is a common feature typically observed in crossply laminated composites comprising of 0 and 90 unidirectional composite layers. Since orthogonally woven composites consist of warp yarns (0 ) and weft yarns (90 ) and the individual yarns can be treated as unidirectional composites, understanding of damage mechanisms in the latter can be useful in designing orthogonal woven composites. Although continuum damage models are suggested and able to capture the nonlinear behavior of composites in certain situations, they are not suitable for modeling the discrete characteristics of damage process in the present study [Wisnom (2010)]. Hence the matrix cracks and delaminations are usually modeled discretely in order to study their interactions [Hallett, Jiang, Khan and Wisnom (2008); Zhou, Fang, Cox and Yang (2010)]. Figure 1: (a) Orthogonally woven 3D composite with the SBS setup and (b) Representative Volume Element (RVE) for the FE model Cohesive elements are widely used for modeling of delaminations and matrix cracks because of their versatility in dealing with damage initiation and evolution without defining any precrack [Nishikawa, Okabe and Takeda (2007), Okabe and Yashiro (2012)]. Apart from delaminations which mostly occur at the interfaces between layers, the location and direction of matrix cracks may be arbitrary. The extended finite element method (XFEM) [Belytschko, Cracie, and Ventura (2009)] and the augmented finite element method (AFEM) [Ling, Yang and Cox (2009)] have been used to deal with these arbitrary discontinuities due to cracks in the material system. However, it might be difficult to predict exactly the creation of multiple cracks in
4 70 Copyright 2013 Tech Science Press CMC, vol.35, no.1, pp.6785, 2013 complex material systems such as woven composites as observed in the experiment without considering uncertainties in geometric configurations, internal defects or material properties. Our interest in the present study is focused on the investigation of delamination rather than exact prediction of intralaminar damage attributes in the given material systems. Results from the SBS tests [Walter, Subhash, Sankar and Yen (2010)] provide good guidelines to predict the occurrence of matrix cracks. Then cohesive elements can be used in modeling matrix cracks as well as delaminations. The potential locations for matrix cracks were assumed based on the observation of SBS test specimens and their orientation was determined from the principal (tensile) stress direction in the study. It should be highlighted again that our intention in this paper is to clarify the role of zyarns on delamination in 3D woven composites with different zyarn volume fraction and a 2D plain woven composite. The FE simulations were used to obtain the forcedisplacement relations of various 3D woven composites and to investigate the effect of zyarns on the apparent interlaminar fracture toughness. The relationships between damage patterns and the global response observed in the SBS tests are also explained using the FE results. 2 Finite element model 2.1 3D woven composites The microstructure of the specimens and their boundary conditions in the FE models were based on the experimental studies reported by Walter et al. [Walter, Subhash, Sankar and Yen (2010)]. The geometric parameters of the DY3W such as yarn dimensions and yarn spacing were determined from the micrographs of the 3D orthogonal woven composite [Walter, Subhash, Sankar and Yen (2010)] and summarized in Table 1. As shown in Figs. 1 and 2 the crosssections of the yarns were treated as rectangles. Due to symmetry about the yzplane passing through the midspan, only onehalf of the specimen in the xdirection was modeled. Since the specimen was assumed to be under a state of plane strain normal to the yaxis, one unitcell in the width direction (ydirection) should be sufficient. Further reduction could be made as the unitcell is symmetric about its midplane parallel to the xzplane. Thus, only one half of the unitcell needs to be considered as shown in Fig. 1(b). The indenter and supports of the SBS test setup were modeled as rigid bodies. The span of the beam (distance between the supports) in the FE model was 40 mm. The thickness of the zyarn in the SY3W was 0.4 mm, half of that in the DY3W. Apart from altering the thickness of the zyarn in the SY3W other geometric dimensions remained the same in the SY3W and the DY3W specimens. In addition, the regions created by reducing the thickness of the zyarn were replaced by matrix
5 Finite Element Analysis of Delamination 71 material since more matrix regions in the SY3W were observed in the micrograph of the specimens [Walter, Subhash, Sankar and Yen (2010)]. Table 1: Dimensions of geometric model of the RVE in mm units [17]. The subscripts x, y and z indicate warp yarn, weft yarn and z yarn, respectively. L s w z t x t y t z w y t g Plane strain boundary conditions were assigned on the front and back surface of 3D woven composites (x z planes in Fig.1) as well as the symmetry boundary conditions on the symmetry plane such that U x =0 (left y z plane in Fig.1). Eightnodes brick elements were used in modeling the yarns and matrix phase and eightnode cohesive elements were used for damage modeling. Considering linear elastic behavior of the yarns and matrix, elastic constants of the yarns were computed using the micromechanics formulas developed by Chamis et al. [Chamis, Handler and Manderscheid (2007)]. The yarns were comprised of S2 glass fiber (Elastic modulus of 86.9GPa and Poisson s ratio of 0.23) and SC15 epoxy along with 62% fiber volume fraction. The strength and critical energy release rate values for the cohesive elements were selected from the literature [Walter, Subhash, Sankar and Yen (2010); Advanced Materials (2013); Huang and Waas; Applied Poleramic (2013)]. The material properties of the yarns, the epoxy and the cohesive elements used in the FE models are listed in Table 2. Table 2: Material properties of the constituents in the 3D woven composites [27] Yarns (Transversely isotropic) E 1 (GPa) E 2 (GPa) E 3 (GPa) ν 12 ν 13 ν 23 G 12 (GPa) G 23 (GPa) G 31 (GPa) Epoxy Cohesive element E 370/830 (GPa) 2.7 ν 0.3 Mode I/II Strength (MPa) 23/33 Mode I/II Fracture toughness (N/m)
6 72 Copyright 2013 Tech Science Press CMC, vol.35, no.1, pp.6785, Damage modeland modeling strategy As reported in [Walter, Subhash, Sankar and Yen (2010)] and will be reported later in this paper, during the beginning stage of the SBS tests, 3D woven composite specimens underwent elastic deformation. As the loads increased, matrix cracks and delaminations developed. The cohesive element associated with a bilinear tractionseparation law was selected for modeling both matrix cracks and delaminations. This damage law enables the traction between two surfaces to be expressed in terms of relative displacement and stiffness: σ = (1 D)Kd 0, d < d 0 d f (d d 0 ) D = d(d, d f d 0) 0 < d < d f 1, d f < d (1) where σ is the traction, K is stiffness, D is the damage variable, d is displacement, d is the displacement at damage initiation and d f is the final displacement [Camanho, Dávila and de Moura (2003)] Quadratic stressbased failure criterion and mixed mode strain energy release rate criterion were used for damage initiation and propagation, respectively, for both the matrix cracks and delaminations: { } < σn > 2 { } 2 σs + = 1 (2) { GI σ o n G IC } + { GII G IIC σ o s } = 1 (3) where σ o n and σ o s are interfacial normal and shear strengths, and G IC and G IIC are the Mode I and Mode II critical energy release rates. Since the locations of cohesive elements, which would act as potential crack paths, should be defined a priori, it was necessary to predict reasonably the locations of expected cracks. The prediction for delaminations is straightforward as it would occur between adjacent plies or layers, while that for matrix crack is complex. Based on experimental observations by Walter et al. [Walter, Subhash, Sankar and Yen (2010)], some assumptions were made to determine the locations of potential cracks for the efficient use of cohesive elements as follows: i) Matrix cracks occur both within the fill tows and in the matrix pocket at the tensile bottom layer; ii) Only a single matrix crack is created and allowed to evolve along the principal stress direction; iii) The crack path is a straightline; and iv) The effect of a matrix crack at the topmost compressive layer on delamination is negligible.
7 Finite Element Analysis of Delamination 73 Figure 2: Geometric parameter of RVE: (a) left side view and (b) front side view Figure 3: Prediction of matrix cracks: The lines indicate potential crack paths (a) Principal stress directions in the tensile region (b) Principal stress directions in the entire regions Formation of matrix cracks on the top layers of the beam required special treatment. In the beginning of loading the top side is under compression and no matrix cracks form. However, after delaminations initiated, there was a redistribution of stresses and the delaminated top layers develop tensile stresses and they became sites for initiation of matrix cracks. These locations were identified by analyzing principal stress directions from a preliminary FE analysis. Using the specimen without any damage (see Fig. 2) the principal directions at the centers of fill tows in the tensile region were found. In the subsequent FE model, cohesive elements for the matrix
8 74 Copyright 2013 Tech Science Press CMC, vol.35, no.1, pp.6785, 2013 cracks were implemented along the principal directions found in the previous step. Other cohesive elements for delaminations were simultaneously placed between layers so that the principal directions in the compressive region after delamination could be found. A similar FE analysis was performed using the specimen of Fig. 3(a) in which the load was applied until delaminations occurred so that redistributed stress fields could be obtained. In order to determine the principal stress directions in the weft yarns, stress values in all elements of the weft yarns were checked and appropriate principal stress directions were chosen for cohesive elements. The principal stress directions determined are shown in Fig. 3(b) over the entire specimen. Note that the angles shown in Fig. 3 were measured from the zaxis. As a result of consecutive finite element simulations the final configuration of Fig. 3(b) was reached which was then used to study of delamination damage of the 3D woven composites. 2.3 Finite element model for 2D plain woven laminates (2DPL) A plain woven laminate (2DPL) with stacking sequence [ (0 pw /45 pw ) 2 / 0 pw] S was also analyzed, where the superscript pw denotes plainwoven. The 2DPL was chosen for comparison with the 3D woven composites, and thus investigating the effect of zyarns on delamination behavior. For the sake of simplicity of FE simulations, each plain woven layer was homogenized as an orthotropic material and onehalf of the beam was modeled using eightnode plane strain elements. The material properties of the homogenized plainwoven layer are listed in Table 3 [Xiao, Gama and Gillespie Jr. (2007)]. The material properties for ±45 pw could be obtained using coordinate transformation. Table 3: Elastic properties for the plain woven composites[34] E 1 =E 2 E 3 G 13 =G 23 G 12 ν 13 = ν 23 ν 12 (GPa) (GPa) (GPa) (GPa) The creation of matrix cracks and placement of cohesive elements in the 2DPL specimens were similar to the procedures used for the 3D woven laminates. Our approach was confirmed by the experimental observation that a single matrix crack tended to occur inside weft yarns of the 0/90 pw [Walter, Subhash, Sankar and Yen (2010)]. However, the tensile cracks in the matrix pocket of outermost layer seen in the 3D woven composites were not observed in plain woven laminates, and hence they were not introduced in the 2DPL specimens. Furthermore, transverse shear stress vanishes at the free surface. Therefore, cohesive elements for possible matrix
9 Finite Element Analysis of Delamination 75 cracks were placed in the three inner homogenized layers of 0/90 pw as shown in Fig. 4. Principal stress directions were found in locations corresponding to the centers of fill tows using the same procedure as in 3D woven composites. The possible matrix crack directions used in this simulation are shown in Fig.4. Figure 4: Implementation of cohesive element on homogenized 2D plain woven composite A parametric study varying Mode I/Mode II interlaminar fracture toughness (370/830 N/m, 1,000/2,000 N/m and 1,000/3,300 N/m) was performed in order to investigate the effect of interlaminar fracture toughness on the global behavior and the evolving damage pattern in 2DPL specimens. These studies were referred to as Case I, Case II and Case III (see Table 4), respectively. Table 4: Parameters for the cohesive element in baseline composite model σ max G Ic τ max G IIc (MPa) (N/m) (MPa) (N/m) Case I Case II Case III Results and discussions 3.1 3D woven composites The force and displacement at the indenter were calculated using the FE simulations. The force for a given displacement could be a proper measure to examine the macroscopic behavior of the specimen. The results for both the SY3W and the
10 76 Copyright 2013 Tech Science Press CMC, vol.35, no.1, pp.6785, 2013 DY3W are shown in Fig.5. Two forcedisplacement curves from the experiments [Walter, Subhash, Sankar and Yen (2010)] are also plotted for comparison. Note the two experimental curves of the same SY3W specimens show slightly different behavior after damage initiation indicating a large variability in specimens. The solid lines indicate the result from the FE model. Since the same properties for the cohesive elements were used and most configurations remained the same except for the thickness of zyarns in the simulation of SY3W and DY3W specimens, it could be inferred that the difference between two FE simulations (solid curves in Fig.5) resulted from the effect of zyarns on delamination. The peak load of the DY3W was higher than that of the SY3W. This revealed that zyarns could delay the damage initiation point. Moreover, the forces beyond the peak loads between the two cases were quite different. The SY3W showed the abrupt forcedrop right after the peak load whereas the forcedrop in the DY3Wwas fairly small. Additionally the SY3W had another peak load followed by the sudden force drop again, which did not occur in the DY3W. These characteristics agree well with experimental results shown in Fig. 5. Figure 5: Forcedisplacement curves of the SY3W and the DY3W The variation of strain energy and damage energy as a function of indenter displacement obtained from the FE analyses are shown in Fig. 6. The strain energy represents the recoverable elastic energy stored in the specimen at any given instant. The damage energy is the unrecoverable energy dissipated by the cohesive elements. It was seen that the sudden forcedrop in the loaddeflection diagram
11 Finite Element Analysis of Delamination 77 corresponded to sudden increase in damage energy. One can note that the damage energy in the DY3W specimen increased steadily without any abrupt damage process or loss of stiffness. From these figures it was clear that zyarns could enhance damage resistance and tolerance. However, optimum amount of z yarn should be used so that there is no deterioration in the inplane properties of the composite [Song, Snakar, Subhash and Yen (2012); Rao, Sankar and Subhash (2009)]. Figure 6: Strain energy and damaged energy versus displacement curves of the SY3W and the DY3W. SE and DE indicate strain energy and damage energy, respectively. 3.2 Plain woven laminated composites Unlike 3D woven composites, only one configuration, but with various cohesive parameters, was considered in studying the 2DPL. Although the same properties for cohesive element as the 3D woven composites were initially used for the 2DPL, interlaminar fracture toughness values would be different since woven laminated composites have higher fracture toughness value than unidirectional fiber composites due to the undulation of yarns or crimps [Kalarikkal, Sankar and Ifju (2006)]. The force versus displacement curves at the indenter due to three different interlaminar fracture toughness values are plotted in Fig. 7. Out of the three sets of interlaminar fracture toughness values used, the forcedisplacement curve of Case III with the highest fracture toughness exhibited loaddisplacement behavior similar to experimental results as shown in Fig.7. Lower fracture toughness values
12 78 Copyright 2013 Tech Science Press CMC, vol.35, no.1, pp.6785, 2013 (cases I and II) resulted in different damage pattern and produced different loaddisplacement curves. Figure 7: Forcedisplacement curves of the 2DPL The distinction among these three forcedisplacement curves is apparent. As the fracture toughness values were increased, the peak loads also increased and the rate of force drop just beyond the peak load became moderate. If the interlaminar cracks propagate mainly without other delaminations the forces will decrease rapidly. As seen in Fig. 7 the rapid force drops in the Case I and Case II were attributed to the damage that occurred with very small increment of displacement and could be clearly identified with the damage energy variation in Fig. 8. Sudden increase of the damage energy was accompanied by sudden loss of the strain energy as well. But the damage energy of Case III increased gradually along with the increase of the strain energy. These variations of global responses were highly dependent on how damage evolved. By observing the history of damage development, it was possible to gain insight into delamination damage behavior of composites. Once delamination occurred from the matrix crack, it would propagate and in the end reach the free end of the specimen (b2and c2 in Fig. 9). The propagation of the crack to the free end caused the force to decrease abruptly. After a complete delamination developed over the region from matrix cracks to the end of the specimen, the force increased with displacement and the strain energy was stored until the state of stress in another interlaminar region satisfied with the criterion for crack initiation and propagation. Then the force would decrease suddenly again
13 Finite Element Analysis of Delamination 79 Figure 8: Strain energy and damage energy versus displacement curves of the 2DPW. SE and DE indicate strain energy and damage energy, respectively. Figure 9: Damage evolution of the 2DPL  Case I: (a) d=0.8mm (b) d=1.1mm (c) d=1.7 mm
14 80 Copyright 2013 Tech Science Press CMC, vol.35, no.1, pp.6785, 2013 Figure 10: Damage evolution of the 2DPL  Case II: (a) d=1mm (b) d=1.5mm (c) d=1.75 mm Figure 11: Damage evolution of the 2DPL  Case III: (a) d=1mm (b) d=1.5mm (c) d=1.75 mm
15 Finite Element Analysis of Delamination 81 Figure 12: Delamination patterns in the composites: (a) the 2DPL (b) the SY3W (c) the DY3W as shown in the Case I of Figs. 7 and 9(c). Case II showed that the resistance to crack propagation increased with the interlaminar fracture toughness. Although the interlaminar crack was created from a matrix crack at a different location from the Case I and propagated up to the end of the specimen, there was a region where the rate of force drop became slow (Fig. 7). Further increase in interlaminar fracture toughness (Case III) changed the tendency of crack propagation totally. High resistance against cracks kept the interlaminar delamination from propagating. Before a delamination reached to the end of specimen, another delamination occurred. This caused a gradual force drop instead of an abrupt drop in the Case I and II (Figs. 7 and 11). The relationships between the damage patterns in Figs. 9 through 11 and the forcedisplacement curves in Fig. 7 were similar to the test results of Walter [Walter (2011)]. It could be observed that the crack propagation of the SY3W reached the end of the specimen and resulted in the forcedisplacement curve in Fig. 5, while the 2DPL and the DY3W didn t allow delaminations to propagate to the end of the specimens or other delaminations occurred at the same time and thus they resulted in gradual force drop as shown in Fig 12. It should be noted that Fig. 12 has been obtained from low velocity impact tests but exhibited similar damage patterns as quasistatic tests demonstrating that quasistatic indentation tests could provide insight into damage development due to impact loading in laminated 3D composites. From these results, it was possible to identify the role of zyarns on delamina
16 82 Copyright 2013 Tech Science Press CMC, vol.35, no.1, pp.6785, 2013 tion. Zyarns provided constraints to reduce the relative displacement between two layers, thus enhancing the resistance against crack propagation. Thus the zyarns resulted in higher apparent interlaminar fracture toughness. 4 Summary and Conclusions The effect of zyarns on damage tolerance of 3D woven composites was studied by simulating the Short Beam Shear test specimens. Based on the previous experimental observations that tensile or transverse matrix cracks develop in the matrix pocket between zyarn crowns and inside wept yarns, a simplified FEM approach using cohesive elements was introduced. The cohesive elements associated with bilinear damage model were placed along the principal stress direction for the matrix cracks and between layers for delaminations. The FE model incorporating RVE model and plane strain boundary condition provided reasonable results to understand the role of zyarns and inherent interlaminar fracture toughness. From the FE simulations of the SY3W and the DY3W specimens, it was found that appropriate volume fraction of zyarns could enhance the damage resistance and tolerance by preventing two neighboring layers from being separated. These conclusions agreed well with the result from the endnotch flexure (ENF) specimen of 3D woven composites by Pankow et al. [Pankaw, Waas, Yen and Ghiorse (2011)]. In the case of the 2DPL, crimps or undulations would interrupt the propagation of delamination cracks providing better damage tolerance than the SY3W where the volume fraction of zyarn is insufficient. However, the DY3W had superior damage tolerance compared to the 2DPL and the SY3W. From the parametric study for the 2DPL, it was concluded that the prevention of crack growth along an entire interface without other damages was a key factor in enhancing damage tolerance. When damages occurred in different layers before the delamination propagated in the entire specimen, more energy was dissipated in various interlaminar damage mechanisms thus increasing the damage tolerance of the laminated composite structure. Finally, the FE models for two types of 3D woven composites and a parametric study for 2D plain woven composites provided a good correlation between the amount of zyarns and interlaminar fracture toughness They help in the understanding of role of zyarn in enhancing apparent fracture toughness, which would be very practical in the design of composite structures. Acknowledgements The funding for this work was provided by the United States Army Research Office (grant number W911NF ) and the United States Army Research Labo
17 Finite Element Analysis of Delamination 83 ratory. The authors also would liketo thank Dr. Bazle Z. (Gama) Haque at the University of Delaware for the personal communication about the volume fraction of yarns in 3D woven composites. References Advanced Materials (2013): Applied Poleramic. (2013): Belytschko, T.; Cracie, R.; Ventura, G. (2009): A review of extended/generalized finite element methods for material modeling. Modeling Simulation Material Sci Eng, vol.17, no.4, pp Byrd, L.W.; Birman, V. (2005): The estimate of the effect of zpins on the strain release rate,fracture and fatigue in a composite cocured zpinned double cantilever beam. CompositeStructures, vol.68, pp Camanho, P.P.; Dávila, C.G.; de Moura, M.F. (2003): Numerical simulation of mixedmode progressive delamination in composite materials. J Composite Material, vol.37, no.16, pp Cartie D.D.R. (2000): Effect of Zfibreson the delamination behaviour of carbonfibre/epoxy Laminates Ph.D.thesis, Cranfield University, UK. Chamis, C.C.; Handler, L.M.; Manderscheid, J. (2007): Composite Nanomechanics: A Mechanistic Properties Prediction. NASA/TM , Glenn Research Center, Cleveland, OH. Chen,L; Sankar, B.V.; Ifju, P.G. (2002): A new mode I fracture test for composites with translaminar reinforcements. Composites Science & Technology, vol.62, pp Dantuluri, V; Maiti, S; Geubelle, P.H.; Patel, R.; Kilic. H. (2007): Cohesive modeling of delamination in Zpin reinforced composite laminates. Composites Science & Technology, vol.67, pp Grassi, M; Zhang, X. (2003): Finite element analyses of mode I interlaminar delamination in zfibre reinforced composite laminates. Composites Science & Technology, vol.63, pp Hallett, SR.; Jiang, WG.; Khan, B.; Wisnom, MR (2008): Modelling the interaction between matrix cracksand delamination damage in scaled quasiisotropic specimens. Composites Science & Technology, vol.68, pp Huang, H.; Waas, A.M. (2009): Compressive response of Zpinned woven glass fiber textile composite laminates: Modeling and computations. Composite Science
18 84 Copyright 2013 Tech Science Press CMC, vol.35, no.1, pp.6785, 2013 & Technology, vol.69, no.14, pp Jain L.K.; Mai Y.W. (1998): On the effect of stitching on Mode I delamination toughness of laminated composites. Composites Science & Technology, vol.58, pp Kalarikkal S.; Sankar BV.; Ifju PG. (2006): Effect of Cryogenic Temperature on the Fracture Toughness of Graphite/Epoxy Composites. ASME Journal of Engineering Materials and Technology, vol.128, no.2, pp Ling, D.S.; Yang,Q.D.; Cox, B. (2009): An augmented finite element method formodeling arbitrary discontinuities in composite materials. Intl J Fracture, vol.156, pp Mabson, GE.; Deobald, LR. (2000): Design curves for 3D reinforcement laminated double cantilever beams. Proc of ASME Int. Mechanical Eng. Congress and Expo., pp Nishikawa, M.; Okabe, T.; Takeda, N. (2007): Numerical simulation of interlaminar damage propagationin CFRP crossply laminates under transverse loading. International Journal of Solids and Structures, vol.44, pp Okabe, T.; Yashiro, S. (2012): Damage detection in holed composite laminates using an embedded FBG sensor. Composites Part A, vol.43, pp Pankow M, Waas AM, Yen CF, Ghiorse S (2011): Resistance to delamination of 3D woven textile composites evaluated using End Notch Flexure (ENF) tests: Cohesive zone based computational results Composites Part A, vol.42, no.12, pp Ratcliffe, J,G.;O brien, T.K. (2004): Discrete spring model for predicting delamination growth in zfiber reinforced DCB specimens. NASA/TM , ARLTR Rao, M.P.; Sankar, B.V.; Subhash, G. (2009): Effect of zyarns on the stiffness and strength of threedimensional woven composites. Composites Part B, vol.40, pp Ratcliffe, J,G.; O brien, T.K. (2004): Discrete spring model for predicting delamination growth in zfiber reinforced DCB specimens. NASA/TM , ARLTR Ratcliffe, J.G.; Kruger, R.A. (2006): Finite Element Analysis for Predicting Mode IDominated Delamination Growth in Laminated Structure with Through Thickness Reinforcement. In: Proceedings of American Society for Composites 21 st Annual Technical Conference, Dearborn, Michigan. Robinson, P.; Das, S. (2004): Mode I DCB testing of composite laminates reinforced with zdirection pins: A simple model for the investigation of data reduction
19 Finite Element Analysis of Delamination 85 strategies. Engg. Fracture Mech, vol.71, pp Sankar, B.V.; Sun, C.T. (1986): LowVelocity Impact Damage in GraphiteEpoxy Laminates Subjected to Tensile Initial Stresses. AIAA Journal, vol.24, no.3, pp Sankar, B.V., Hu, S. (1991): Dynamic delamination propagation in composite beams, J Composite Materials, vol.25, no.11, pp Sankar, B.V.; Sharma, S,K. (1997): Mode II delamination toughness of stitched graphite/epoxy textile composites. Composites Science &Technology, 57, pp Sankar, B.V.;Dharmapuri, S.M. (1998): Analysis of a Stitched Double Cantilever Beam. J Composite Materials, vol.32, pp Sankar, B.V.; Zhu, H. (2000): Effect of stitching on the lowvelocity impact response of delaminated composite beams. Composites Science & Technology, vol.60, pp Song, M.C.; Sankar, B.V.; Subhash, G.; Yen, C.F. (2012): Analysis of mode I delamination of zpinned composites using a nondimensional analytical model. Composites Part B, vol.43, pp Sridhar, N.; Massabo, R.; Cox, B.N.; Beyerlein, I.J. (2002): Delamination dynamics in throughthickness reinforced laminates with application to DCB specimen delaminated composite beams. Int J Fracture, vol.118, pp Walter, T.R.; Subhash, G.; Sankar, B.V.; Yen, C.F. (2010): Monotonic and cyclic short beam shear response of 3D woven composites. Composites Science & Technology, vol.70, pp Walter T.R. (2011): Characterization of delamination in 3d woven composites under static and dynamic loading. PhD thesis. Univ. of Florida Wisnom, M.R. (2010): Modelling discrete failures in composites with interface elements. Composites PartA, vol.41, pp Xiao,JR.;Gama,B.A.;Gillespie Jr., JW (2007): Progressive and delamination delamination in plain weave S2 glass/sc15 composites under quasistatic punchshear loading. Composite Structures, vol.78, pp Zhou, Z.Q.; Fang, X.J.; Cox, B.N.; Yang, Q.D. (2010): The evolution of a transverse intraply crack coupled to delamination cracks. Intl J Fracture, vol.165, pp
20
Composites: Part B. Analysis of mode I delamination of zpinned composites using a nondimensional analytical model
Composites: Part B 43 (2012) 1776 1784 Contents lists available at SciVerse ScienceDirect Composites: Part B journal homepage: www. elsevier. com/ locate/ compositesb Analysis of mode I delamination of
More informationNUMERICAL INVESTIGATION OF DELAMINATION IN LSHAPED CROSSPLY COMPOSITE BRACKET
NUMERICAL INVESTIGATION OF DELAMINATION IN LSHAPED CROSSPLY COMPOSITE BRACKET M.Gümüş a*, B.Gözlüklü a, D.Çöker a a Department of Aerospace Eng., METU, Ankara, Turkey *mert.gumus@metu.edu.tr Keywords:
More informationAutodesk Helius PFA. Guidelines for Determining Finite Element Cohesive Material Parameters
Autodesk Helius PFA Guidelines for Determining Finite Element Cohesive Material Parameters Contents Introduction...1 Determining Cohesive Parameters for Finite Element Analysis...2 What Test Specimens
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationUniversity of Bristol  Explore Bristol Research. Early version, also known as preprint
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 12291245. DOI: 10.1177/0021998305057432
More informationFLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION N. V. De Carvalho 1*, B. Y. Chen
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationCHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS
Oral Reference Number: ICF100942OR CHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS T. Kevin O Brien U.S. Army Research Laboratory Vehicle Technology Directorate
More informationPrediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads
Prediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads J. Raju 1*, D.S. Sreedhar 2, & C.M. Manjunatha 1 1
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationINITIATION AND PROPAGATION OF FIBER FAILURE IN COMPOSITE LAMINATES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS INITIATION AND PROPAGATION OF FIBER FAILURE IN COMPOSITE LAMINATES E. Iarve 1,2*, D. Mollenhauer 1, T. Breitzman 1, K. Hoos 2, M. Swindeman 2 1
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationCOMPARISON OF COHESIVE ZONE MODELS USED TO PREDICT DELAMINATION INITIATED FROM FREEEDGES : VALIDATION AGAINST EXPERIMENTAL RESULTS
COMPARISON OF COHESIVE ZONE MODELS USED TO PREDICT DELAMINATION INITIATED FROM FREEEDGES : VALIDATION AGAINST EXPERIMENTAL RESULTS A. Uguen 1, L. Zubillaga 2, A. Turon 3, N. Carrère 1 1 Laboratoire Brestois
More informationInterlaminar fracture characterization in composite materials by using acoustic emission
5th International Symposium on NDT in Aerospace, 1315th November 2013, Singapore Interlaminar fracture characterization in composite materials by using acoustic emission Ian SILVERSIDES 1, Ahmed MASLOUHI
More informationSSRG International Journal of Mechanical Engineering (SSRGIJME) volume1 issue5 September 2014
Finite Element Modeling for Delamination Analysis of Double Cantilever Beam Specimen Mohammed Waseem H.S. 1, Kiran Kumar N. 2 1 Post Graduate Student, 2 Asst. Professor Dept. of Mechanical Engineering,
More informationADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF COMPOSITES
NAFEMS WORLD CONGRESS 13, SALZBURG, AUSTRIA ADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF M. Bruyneel, J.P. Delsemme, P. Jetteur (LMS Samtech, Belgium); A.C. Goupil (ISMANS, France). Dr. Ir. M. Bruyneel,
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationNumerical Simulation of the Mode I Fracture of Angleply Composites Using the Exponential Cohesive Zone Model
Numerical Simulation of the Mode I Fracture of Angleply Composites Using the Exponential Cohesive Zone Model Numerical Simulation of the Mode I Fracture of Angleply Composites Using the Exponential Cohesive
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationID1160 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING
ID116 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING K. Minnaar and M. Zhou = School of Mechanical Engineering Georgia Institute
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationNumerical Evaluation of Fracture in Woven Composites by Using Properties of Unidirectional Type for modelling
J. Basic. Appl. Sci. Res., 2(12)1320213209, 2012 2012, TextRoad Publication ISSN 20904304 Journal of Basic and Applied Scientific Research www.textroad.com Numerical Evaluation of Fracture in Woven Composites
More informationNumerical Analysis of Delamination Behavior in Laminated Composite with Double Delaminations Embedded in Different Depth Positions
Numerical Analysis of Delamination Behavior in Laminated Composite with Double Delaminations Embedded in Different Depth Positions Numerical Analysis of Delamination Behavior in Laminated Composite with
More informationDAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS DAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT A. Yoshimura 1*, T. Okabe, M. Yamada 3, T. Ogasawara 1, Y. Tanabe 3 1 Advanced
More informationOverview of Probabilistic Modeling of Woven Ceramic Matrix Composites ABSTRACT
ABSTRACT An overview of current research efforts in understanding the cause of variability in the thermomechanical properties of woven ceramic matrix composites is presented. Statistical data describing
More informationDYNAMIC DELAMINATION OF AERONAUTIC STRUCTURAL COMPOSITES BY USING COHESIVE FINITE ELEMENTS
DYNAMIC DELAMINATION OF AERONAUTIC STRUCTURAL COMPOSITES BY USING COHESIVE FINITE ELEMENTS M. Ilyas, F. Lachaud 1, Ch. Espinosa and M. Salaün Université de Toulouse, ISAE/DMSM, 1 avenue Edouard Belin,
More informationDESIGNING DYNAMIC TESTS TO ASSESS RATE DEPENDENCE IN LARGESCALE CRACK BRIDGING
DESIGNING DYNAMIC TESTS TO ASSESS RATE DEPENDENCE IN LARGESCALE CRACK BRIDGING C. LundsgaardLarsen, 1 R. Massabò, 2 and B. N. Cox 3 1 Technical University of Denmark, Lyngby, Denmark 2 DICAT, University
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of Materials Science and Engineering A 6 () 354 doi:.765/663/6..5 D DAVID PUBLISHING Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K * and V V Subba Rao Faculty
More informationThe Effects of Transverse Shear on the Delamination of EdgeNotch Flexure and 3Point Bend Geometries
The Effects of Transverse Shear on the Delamination of EdgeNotch Flexure and 3Point Bend Geometries M. D. Thouless Department of Mechanical Engineering Department of Materials Science & Engineering University
More informationPrediction of Elastic Constants on 3D Fourdirectional Braided
Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Liang Dao Zhou 1,2,* and Zhuo Zhuang 1 1 School of Aerospace,
More informationRandom FiberMatrix Model for Predicting Damage in Multiscale Analysis of Textile Composites under Thermomechanical Loads
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Random FiberMatrix Model for Predicting Damage in Multiscale Analysis of Textile Composites under Thermomechanical Loads W. R. McLendon, J. D.
More informationOn characterising fracture resistance in modei delamination
9 th International Congress of Croatian Society of Mechanics 1822 September 2018 Split, Croatia On characterising fracture resistance in modei delamination Leo ŠKEC *, Giulio ALFANO +, Gordan JELENIĆ
More informationDynamic analysis of Composite Micro Air Vehicles
Dynamic analysis of Composite Micro Air Vehicles Shishir Kr. Sahu Professor and Head, Civil Engineering, National Institute of Technology, Rourkela, India Email: sksahu@nitrkl.ac.in ABSTRACT The present
More informationInteraction of Zpins with multiple mode II delaminations in composite laminates
Interaction of Zpins with multiple mode II delaminations in composite laminates Mehdi Yasaee *, Galal Mohamed, Stephen R. Hallett School of Aerospace, Transport and Manufacturing, Cranfield University,
More informationSimulation of Dynamic Delamination and Mode I Energy Dissipation
Simulation of Dynamic Delamination and Mode I Energy Dissipation Muhammad Ilyas, Christine Espinosa 1, Frédéric Lachaud and Michel Salaün Université de Toulouse ISAE, DMSM, 1 Avenue Edouard Belin, 3154
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationPROGRESSIVE DAMAGE ANALYSES OF SKIN/STRINGER DEBONDING. C. G. Dávila, P. P. Camanho, and M. F. de Moura
PROGRESSIVE DAMAGE ANALYSES OF SKIN/STRINGER DEBONDING C. G. Dávila, P. P. Camanho, and M. F. de Moura Abstract The debonding of skin/stringer constructions is analyzed using a stepbystep simulation
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationFracture Behaviour of FRP CrossPly Laminate With Embedded Delamination Subjected To Transverse Load
Fracture Behaviour of FRP CrossPly Laminate With Embedded Delamination Subjected To Transverse Load Sriram Chintapalli 1, S.Srilakshmi 1 1 Dept. of Mech. Engg., P. V. P. Siddhartha Institute of Technology.
More informationImpact and Crash Modeling of Composite Structures: A Challenge for Damage Mechanics
Impact and Crash Modeling of Composite Structures: A Challenge for Damage Mechanics Dr. A. Johnson DLR Dr. A. K. Pickett ESI GmbH EUROPAM 99 Impact and Crash Modelling of Composite Structures: A Challenge
More informationMulti Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala
Multi Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala Abstract: FRP laminated composites have been extensively used in Aerospace and allied industries
More informationA 3D Discrete Damage Modeling Methodology for Abaqus for Fatigue Damage Evaluation in Bolted Composite Joints
A 3D Discrete Damage Modeling Methodology for Abaqus for Fatigue Damage Evaluation in Bolted Composite Joints Eugene Fang 1, Ling Liu 1, Michael Stuebner 1, Jim Lua 1 1 Global Engineering and Materials,
More informationEffect of Thermal Stresses on the Failure Criteria of Fiber Composites
Effect of Thermal Stresses on the Failure Criteria of Fiber Composites Martin Leong * Institute of Mechanical Engineering Aalborg University, Aalborg, Denmark Bhavani V. Sankar Department of Mechanical
More informationA SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST
A SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST P. Robinson The Composites Centre, Department of Aeronautics, Imperial College London South Kensington, London, SW7 2AZ, UK p.robinson@imperial.ac.uk
More informationNUMERICAL AND EXPERIMENTAL ANALYSES OF MULTIPLE DELAMINATIONS IN CURVED COMPOSITE LAMINATES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS NUMERICAL AND EXPERIMENTAL ANALYSES OF MULTIPLE DELAMINATIONS IN CURVED COMPOSITE LAMINATES A. Baldi 1 *, A. Airoldi 1, P. Belotti 1, P. Bettini
More informationREPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 REPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
More informationIMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS OBTAINED WITH LMS SAMTECH SAMCEF
V ECCOMAS Thematic Conference on the Mechanical Response of Composites COMPOSITES 015 S.R. Hallett and J.J.C. Remmers (Editors) IMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS
More informationFracture Mechanics, Damage and Fatigue: Composites
University of Liège Aerospace & Mechanical Engineering Fracture Mechanics, Damage and Fatigue: Composites Ludovic Noels Computational & Multiscale Mechanics of Materials CM3 http://www.ltascm3.ulg.ac.be/
More informationComposites Part A: Applied Science and Manufacturing 38 (2007) ON THE DELAMINATION SUPPRESSION IN STRUCTURAL JOINTS BY ZFIBRE PINNING
Composites Part A: Applied Science and Manufacturing 38 (2007) 1107 1115. ON THE DELAMINATION SUPPRESSION IN STRUCTURAL JOINTS BY ZFIBRE PINNING G. Allegri, X. Zhang School of Engineering, Cranfield University,
More informationFRACTURE MECHANICS OF COMPOSITES WITH RESIDUAL STRESSES, TRACTIONLOADED CRACKS, AND IMPERFECT INTERFACES
Proc. 2 nd ESIS TC4 Conference on Polymers and Composites, in press, 1999 Author prepared reprint FRACTURE MECHANICS OF COMPOSITES WITH RESIDUAL STRESSES, TRACTIONLOADED CRACKS, AND IMPERFECT INTERFACES
More informationMODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE
MODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE Jean Paul Charles, Christian Hochard,3, Pierre Antoine Aubourg,3 Eurocopter, 375 Marignane cedex, France Unimeca, 6 rue J. Curie, 3453
More informationFailure Analysis of Unidirectional Composite Pinned Joints
217 IJEDR Volume, Issue 4 ISSN: 23219939 Failure Analysis of Unidirectional Composite Pinned Joints 1 Sai Ashok.M, 2 Mr. U. Koteswara Rao 1 Mtech Machine Design, 2 Associate Professor & Asst. COE 1
More informationInsitu local strain measurement in textile composites with embedded optical fibre sensors
Insitu local strain measurement in textile composites with embedded optical fibre sensors S. Daggumati, E. Voet, I. De Baere, W. Van Paepegem & J. Degrieck Ghent University, Department of Materials Science
More informationA Stress Gradient Failure Theory for Textile Structural Composites. Final Technical Report submitted to ARO
A Stress Gradient Failure Theory for Textile Structural Composites Final Technical Report submitted to ARO By RYAN KARKKAINEN and BHAVANI SANKAR University of Florida Department of Mechanical & Aerospace
More informationID1274 SPLIT ANGLEPLY BEAM SPECIMEN FOR MEASUREMENT OF FRACTURE TOUGHNESS WITH MODE III STRESS STATE
ID1274 SPLIT ANGLEPLY BEAM SPECIMEN FOR MEASUREMENT OF FRACTURE TOUGHNESS WITH MODE III STRESS STATE Kunigal Shivakumar, Srikant Ghantae * and Matthew Sharpe Center for Composite Materials Research North
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationParametric Investigation of Gas Permeability in CrossPly Laminates Using Finite Elements
AIAA JOURNAL Vol. 45, No. 4, April 7 Parametric Investigation of Gas Permeability in CrossPly Laminates Using Finite Elements Jianlong Xu and Bhavani V. Sankar University of Florida, Gainesville, Florida
More informationPrediction of impactinduced delamination in crossply composite laminates using cohesive interface elements
Prediction of impactinduced delamination in crossply composite laminates using cohesive interface elements F. Aymerich, F. Dore, P. Priolo To cite this version: F. Aymerich, F. Dore, P. Priolo. Prediction
More informationMESOSCALE MODELLING IN THERMOPLASTIC 5HARNESS SATIN WEAVE COMPOSITE
MESOSCALE MODELLING IN THERMOPLASTIC 5HARNESS SATIN WEAVE COMPOSITE S. Daggumati a*,i. De Baere a, W. Van Paepegem a, J. Degrieck a, J. Xu b, S.V. Lomov b, I. Verpoest b a Ghent University, Dept. of
More informationStressstrain response and fracture behaviour of plain weave ceramic matrix composites under uniaxial tension, compression or shear
Xi an 225 th August 217 Stressstrain response and fracture behaviour of plain weave ceramic matrix composites under uniaxial tension compression or shear Heyin Qi 1 Mingming Chen 2 Yonghong Duan 3 Daxu
More informationEVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationCharacterization of Fiber Bridging in Mode II Fracture Growth of Laminated Composite Materials
Applied Mechanics and Materials Online: 20100630 ISSN: 16627482, Vols. 2425, pp 245250 doi:10.4028/www.scientific.net/amm.2425.245 2010 Trans Tech Publications, Switzerland Characterization of Fiber
More informationDiscrete Spring Model for Predicting Delamination Growth in ZFiber Reinforced DCB Specimens
NASA/TM2004213019 ARLTR3190 Discrete Spring Model for Predicting Delamination Growth in ZFiber Reinforced DCB Specimens James G. Ratcliffe National Research Council Langley Research Center, Hampton,
More informationCalibration and Experimental Validation of LSDYNA Composite Material Models by Multi Objective Optimization Techniques
9 th International LSDYNA Users Conference Optimization Calibration and Experimental Validation of LSDYNA Composite Material Models by Multi Objective Optimization Techniques Stefano Magistrali*, Marco
More informationANALYSIS OF LOAD FLOW AND STRESS CONCENTRATIONS IN TEXTILE COMPOSITES
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS ANALYSIS OF LOAD FLOW AND STRESS CONCENTRATIONS IN TEXTILE COMPOSITES Deepak Goyal*, John D. Whitcomb*, Julian Varghese* *Department of Aerospace Engineering,
More informationKeywords: CFRP, compressive failure, kinkband, cohesive zone model. * Corresponding author
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS AN EXPERIMENTAL METHOD TO DETERMINE THE CRITICAL ENERGY RELEASE RATE ASSOCIATED WITH LONGITUDINAL COMPRESSIVE FAILURE IN CFRP D. Svensson 1 *,
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationModelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations
Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations W. Van Paepegem *, I. De Baere and J. Degrieck Ghent
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationEffects of Resin and Fabric Structure
Fatigue of Wind Blade Laminates: Effects of Resin and Fabric Structure Details David Miller, Daniel D. Samborsky and John F. Mandell Montana State t University it MCARE 2012 Outline Overview of MSU Fatigue
More informationNumerical analysis of the mechanical response of wood glulam beams reinforced through the thickness by FRP rods.
Numerical analysis of the mechanical response of wood glulam beams reinforced through the thickness by FRP rods. Giuseppe Giambanco 1, Tiziana Turetta 1, Alessia Cottone 1 1 Department of Structural, Aerospace
More informationPERFORMANCE OF COMPOSITE PANELS SUBJECTED TO UNDERWATER IMPULSIVE LOADING
PERFORMANCE OF COMPOSITE PANELS SUBJECTED TO UNDERWATER IMPULSIVE LOADING F. Latourte, D. Grégoire, R. BellurRamaswamy, H.D. Espinosa* Northwestern University, 2145 Sheridan Road, Evanston IL 60202 (*)
More informationSKINSTRINGER DEBONDING AND DELAMINATION ANALYSIS IN COMPOSITE STIFFENED SHELLS
SKINSTRINER DEBONDIN AND DELAMINATION ANALYSIS IN COMPOSITE STIFFENED SHELLS R. Rikards, K. Kalnins & O. Ozolinsh Institute of Materials and Structures, Riga Technical University, Riga 1658, Latvia ABSTRACT
More informationMicromechanical analysis of FRP hybrid composite lamina for inplane transverse loading
Indian Journal of Engineering & Materials Sciences Vol. 15, October 2008, pp. 382390 Micromechanical analysis of FRP hybrid composite lamina for inplane transverse loading K Sivaji Babu a *, K Mohana
More informationFrontiers of Fracture Mechanics. Adhesion and Interfacial Fracture Contact Damage
Frontiers of Fracture Mechanics Adhesion and Interfacial Fracture Contact Damage Biology, Medicine & Dentistry The Next Frontiers For Mechanics One of the current challenges in materials & mechanics is
More informationApplication of fracture mechanicsbased methodologies for failure predictions in composite structures
Application of fracture mechanicsbased methodologies for failure predictions in composite structures Zoltan Mikulik a, B. Gangadhara Prusty a, Rodney S. Thomson b, Donald W. Kelly a,* a School of Mechanical
More informationCrashworthiness of composite structures: Experiment and Simulation
Crashworthiness of composite structures: Experiment and Simulation Francesco Deleo, Bonnie Wade and Prof. Paolo Feraboli (UW) Dr. Mostafa Rassaian (Boeing R&T) JAMS 2010 The Joint Advanced Materials and
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationMODE I RATE DEPENDENT MESOMECHANICS OF ZPINS
21 st International Conference on Composite Materials Xi an, 2025 th August 2017 MODE I RATE DEPENDENT MESOMECHANICS OF ZPINS Hussein Hijazi 1, Giuliano Allegri 2, Hao Cui 3 Stephen R. Hallett 4 and
More informationPREDICTION OF OUTOFPLANE FAILURE MODES IN CFRP
PREDICTION OF OUTOFPLANE FAILURE MODES IN CFRP R. R. Pinto 1, P. P. Camanho 2 1 INEGI  Instituto de Engenharia Mecanica e Gestao Industrial, Rua Dr. Roberto Frias, 4200465, Porto, Portugal 2 DEMec,
More informationHIGH VELOCITY IMPACT ON TEXTILE REINFORCED COMPOSITES
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS HIGH VELOCITY IMPACT ON TEXTILE REINFORCED COMPOSITES Warnet L., Akkerman R., Ravensberg M. University of Twente, Faculty of Engineering Technology,
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationMECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING
MECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING Steven Roy, Larry Lessard Dept. of Mechanical Engineering, McGill University, Montreal, Québec, Canada ABSTRACT The design and
More informationDESIGNING A FLEXIBLE BELLOWS COUPLING MADE FROM COMPOSITE MATERIALS USING NUMERICAL SIMULATIONS SVOČ FST 2018
DESIGNING A FLEXIBLE BELLOWS COUPLING MADE FROM COMPOSITE MATERIALS USING NUMERICAL SIMULATIONS SVOČ FST 2018 Ing. Frantisek Sedlacek, University of West Bohemia, Univerzitni 8, 306 14, Pilsen, Czech Republic
More informationStrength of GRPlaminates with multiple fragment damages
Strength of GRPlaminates with multiple fragment damages S. Kazemahvazi, J. Kiele, D. Zenkert Kungliga Tekniska Högskolan, KTH 100 44 Stockholm, Sweden sohrabk@kth.se SUMMARY The strength of glass fibre
More informationCHEME2200: Polymer blends and composites Fibre architecture and principles of reinforcement
CHEME2200: Polymer blends and composites Fibre architecture and principles of reinforcement Mark Hughes 19 th September 2016 Outline Fibre architecture Volume fraction and the rule of mixtures Principle
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationInternational Journal of Innovative Research in Science, Engineering and Technology Vol. 2, Issue 7, July 2013
ANALYSIS AND MITIGATION OF STRESS CONCENTRATION FACTOR OF A RECTANGULAR ISOTROPIC AND ORTHOTROPIC PLATE WITH CENTRAL CIRCULAR HOLE SUBJECTED TO INPLANE STATIC LOADING BY DESIGN OPTIMIZATION Shubhrata Nagpal
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More informationComposite Materials 261 and 262
Composite Materials 261 and 262 Stefan Hartmann 1 David Moncayo 2 1 DYNAmore GmbH, Stuttgart, Germany 2 Daimler AG, Sindelfingen, Germany 11. LSDYNA Forum 2012, 9.  10. Oktober 2012, Ulm 1 Outline Introduction
More informationShear Lag And Beam Theories For Structures
Shear Lag And Beam Theories For Structures B N Cox, M Andrews, R Massabò, 3 A Rosakis, 4 N Sridhar, and Q D Yang Rockwell Scientific Co. LLC, Thousand Oaks, California, U.S.A. Department of Civil and Environmental
More informationBRIDGED DELAMINATION CRACKS IN CURVED BEAMS AND MIXEDMODE BENDING SPECIMENS
BRDGED DELANATON CRACKS N CURVED BEAS AND XEDODE BENDNG SPECENS Roberta assabò and Brian N. Cox Department of Structural and Geotechnical Engineering, University of Genova, Via ontallegro, 645, Genova,
More informationThe numerical simulation research of an UltraLight Photovoltaic Cell multilayer composite structure
5th International Conference on Civil, Architectural and Hydraulic Engineering (ICCAHE 2016) The numerical simulation research of an UltraLight Photovoltaic Cell multilayer composite structure Kangwen
More informationFINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Ever J. Barbero Department of Mechanical and Aerospace Engineering West Virginia University USA CRC Press Taylor &.Francis Group Boca Raton London New York
More information